# Transport Properties of Carbon Nanotubes

```Transport Properties of
Carbon Nanotubes
By: Shaun Ard
Carbon nanotubes are on the forefront of a multitude of exciting research areas.
They offer research opportunities to both the application focused engineer and the
fundamental theorist alike. Of particular interest to this diverse field is the area of
transport through these nanotubes. The unique characteristics of the nanotubes allow for
potential applications into nano-based electronics, as well as offer a simple onedimensional system for the study of fundamental quantum models.
The transport properties of carbon nanotubes are very much dependant on the
exact nature in which it is formed. Therefore, one must start with a proper basis with
which to describe them. It can be defined by a graphene sheet and its familiar hexagonal
unit cell. Two unit vectors &acirc;1 and &acirc;2 are used to form the chiral vector, Ch = n &acirc;1 + m &acirc;2,
which describes how the graphene sheet is “rolled up” to form the nanotubes illustrated in
Figure 11. This chiral vector, or the associated (n,m) index, is used to describe the type of
nanotubes. The important measurables such as helicity and circumference can be
expressed in terms of these indices.
Figure 1. Schematic representation showing the formation of the nanotubes from a graphene sheet
(a). Tubes are classified as armchair (Ba), zigzag (Bb), or chiral (Bc) based on their (n,m) index
(Popov).
One of the more interesting transport properties of nanotubes is the demonstration
of both semi-conducting and metallic properties. This can be explained with a fairly
simple model; since nanotubes are essentially just &quot;rolled up&quot; graphene sheets, then that
is how they are described theoretically. One starts with the 2 dimensional band structure
of graphene, which is well described by a tight binding model. The band structure of the
nanotubes is then derived from &quot;folding&quot; this band structure in a way based on the
chirality and therefore the (n, m) index of the nanotubes, as seen in Figure 2. This model
predicts nanotubes to behave metallically if n-m is evenly divisible by 3, and semiconducting with a finite band gap otherwise. Work done by Odom et al.2 utilized
scanning tunneling microscopy (STM) to probe both the structure and electronic density
of states simultaneously. They found that different nanotubes clearly behaved as either
metals or semiconductors, seemingly in agreement with the predictions based on their
indices.
Advances in growth techniques have allowed for connection of nanotubes to
electrodes for detailed transport study. Semi-conducting tubes have been looked at in this
regard for applications in Field Effect Transistors (FETs). For conducting tubes,
however, this has allowed for study fascinating aspects of low dimensional quantum
effects. Bockrath et al., studied the transport across ropes of single walled nanotubes
(SWNTs) 3,4. Figure 2 shows the I-V measurements of these ropes for a variety of
temperatures. They found significant suppression of the conductance near V=0 for low
temperatures. In addition, the conductance at low temperature (1.3 K) consisted of a
series of sharp peaks that broadened at higher temperatures, when plotted versus gate
voltage as seen in Figure 2. This is due to the electron-electron interaction playing more
of a role in this system. The contacts essentially form a zero dimensional quantum dot
out of the nanotubes, with the electron described well as a particle in a box. These
quantized levels combined with the electron interaction are described as a Coulomb
Blockade, that is prevalent at the low temperatures. The periodicity of the peaks imply
that transport through these ropes is dominated by a single metallic tubes, consistent with
the (n,m) index prediction that most of the tubes would be semi-conductors and thus nonconducting at these temperatures.
Figure 2. I-V plot for different temperatures (left). Conductance versus gate voltage (a) with peaks
The continued work on this subject by Brockath et al highlights the importance of
interactions between electrons in this system. This marks the deviation from the Fermiliquid model typically applied to conductors, to that of a Luttinger-liquid (LL) where
even small Coulomb interactions have a significant impact. In Figure 3, we again see a
plot of conductance versus gate voltage, this time for several temperatures. At low T, we
again see evidence of the Coulomb Blockade, which is then &quot;washed out&quot; as T is
increased. However, this model alone doesn't explain the strong dependence of
conductance on T. Whereas the tunneling amplitude into a Fermi-liquid is expected to be
energy independent, the electron correlation in a LL is expected to vanish as a power law
with respect to energy. This then implies a power law dependence of conductance on T
at low bias, and the bias itself at higher voltages. The inset in Figure 3 shows this power
law dependence on T.
Figure 3. Conductance versus gate voltage for noted temperatures. Temperature dependence of
conductance (inset) (Bockrath).
Further evidence of LL behavior in this system is seen in the differential
conductance behavior with respect to bias voltage. Figure 4 shows this relationship for
different temperatures and is scaled to include them on the same plot. The relationship is
that of a power law at higher bias voltages as predicted for a LL. Additionally, Figure 4
highlights the two different methods of connecting the nanotubes to the electrodes for
these experiments, end and bulk contacted. For this system the contact interface is
crucial and the difference between the contact types is evident in the power law scaling
factors. However, this remains an area for further study to better understand.
Figure 4. Scaled differential conductance versus bias voltage for both bulk contacted (a) and end
contacted (b) (Bockrath).
Other fundamental phenomena are evident in nanotube transport. Babic and
Sch&ouml;nenberger5 did work similar to that previously mentioned. However, they were able
to create very &quot;transparent&quot; connections to the nanotubes with which they could then
control by varying the gate voltage. The differential voltage was then plotted with
respect to both bias and gate voltages. Figure 5 shows this plot and the interesting
physics involved. At high gate voltages there is weak coupling between the nanotubes
and the contacts forming a quantum dot evidenced by the coulomb blockade features
discussed earlier. As the gate voltage is lowered, the contacts become more transparent
and the coupling becomes intermediate. Higher order tunneling terms come in to play
forming Kondo resonances. As the gate voltage is minimized and the coupling
maximized, the quantum dot approaches an open wire. The conductance approaches the
theoretical maximum for a single tube, 4e2/h. However, residual scattering from the
contacts results in the remaining periodicity. Interestingly, sharp resonances arrise that
are well modeled as Fano resonances. The source of the resonant and non-resonant
channels contributing to this Fano resonance are still not well understood. This
experiment provides an example of the different quantum regimes available for study
with carbon nanotubes.
Figure 5. Differential conductance versus bias (Vsd) and gate (Vg) voltages, with the corresponding
linear response conductance underneath (Babic).
Whereas the previously discussed experiments focused on dc electrical transport,
Zhao et al6, looked into frequency dependant transport. Figure 6 shows the multiple
probe set up employed as well as the impedance versus frequency plots measured. They
found that the impedance could be modeled fairly well as an RC circuit with one major
discrepancy; there is a very sharp resonance at 37.6 kHz consistently appearing. Figure
7 shows this resonance remaining for tubes of different lengths. This along with
temperature dependant data leads the authors to believe it is an intrinsic feature to the
nanotubes, but is not well understood beyond that.
Figure 6. Real and imaginary parts of the impedance (dotted) versus frequency for both high
(a,b)and low(c,d) frequency regimes. Additionally, theoretical values (solid) using a R-C circuit
model. Multi-probe setup employed for multiple lengths of tube (e) (Bockrath).
Figure 7. Differential impedances for varying tube lengths showing the consistency of the resonance.
The experiments referenced above are but a sampling of the considerable research
involving transport in carbon nanotubes. Potential application aside, these nanotubes
offer insight into an array of exotic phenomenon. It offers opportunity to both tune
current models and develop new ones. As preparation methods and experimental
techniques evolve our understanding of the most fundamental aspects of physics shall
only improve.
1
V. Popov, Carbon nanotubes: properties and applications, Materials Science and Engineering R 43
(2004) 61-102
2
T.W. Odom, J. Huang, P. Kim, C. Lieber, Atomic Structure and Electronic Properties of Single-Walled
Nanotubes, Nature (London) 391 (1998) 62
3
M. Bockrath, D. Cobden, P. McEuen, N. Chopra, A. Zettl, A. Thess, R. E. Smalley, Single-Electron
Transport in Ropes of Carbon Nanotubes , Science 275 (1997) 1922
4
M. Bockrath, D. Cobden, Jia Lu, A. Rinzler, R. Smalley, L. Balents, P. McEuen, Luttinger-liquid
behaviour in carbon nanotubes, Nature 397 (1999) 598
5
B. Babic and C. Sch&ouml;nenberger, Observation of Fano resonances in single-wall carbon nanotubes, Phys.
Rev. B 70 (2004) 195408
6
Y. Zhao, B. Wei, P. Ajayan, G. Ramanath, T. Lu, G. Wang, A. Rubio, S. Roche, Frequency-dependent
electrical transport in carbon nanotubes, Phys. Rev. B 64 (2001) 201402-1
```